View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
Designation: A 121 – 99 AMERICAN SOCIETY FOR TESTING AND MATERIALS 100 Barr Harbor Dr., West Conshohocken, PA 19428 Reprinted from the Annual Book of ASTM Standards. Copyright ASTM Standard Speciﬁcation for Metallic-Coated Carbon Steel Barbed Wire1 This standard is issued under the ﬁxed designation A 121; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (e) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense.1. Scope MIL-STD-129 Marking for Shipment and Storage4 1.1 This speciﬁcation covers metallic-coated steel barbed MIL-STD-163 Steel Mill Products Preparation for Ship-wire, consisting of a strand of two wires. ment and Storage4 1.2 The barbed wire is available with aluminum, zinc, and 3. Terminologyzinc-5 % aluminum-mischmetal alloy coatings, with a numberof coating weights, in a number of different constructions 3.1 Deﬁnitions—For deﬁnitions of terms used in this speci-(designs), and in two grades. Not all designs are available in all ﬁcation, refer to Terminology A 902.coating types. 4. Classiﬁcation 1.3 The values stated in inch-pound units are to be regardedas the standard. The values given in parentheses are for 4.1 The barbed wire covered by this speciﬁcation is classi-information only. ﬁed as described in this section. 1.4 The text of this speciﬁcation references notes and 4.2 Design Number—Numbers describing standard sizesfootnotes that provide explanatory information. These notes and constructions, as listed in Table 1.and footnotes (excluding those in tables) shall not be consid- 4.3 Metallic Coating Type:ered as requirements of the speciﬁcation. 4.3.1 Coating Type A—Made from aluminum-coated strand wire.2. Referenced Documents 4.3.2 Coating Type Z—Made from zinc-coated strand wire. 2.1 ASTM Standards: 4.3.3 Coating Type ZA—Made from zinc-5 % aluminum- A 90/A 90M Test Method for Weight (Mass) of Coating on mischmetal alloy (Zn-5AL-MM) coated strand wire. Iron and Steel Articles with Zinc or Zinc-Alloy Coatings2 4.4 Metallic Coating Class—The speciﬁed amount of coat- A 428/A 428M Test Method for Weight of Coating on ing (coating weight [mass]) on the strand wire. Aluminum-Coated Iron or Steel Articles2 4.4.1 For Coating Type A, see 6.3. (Only one coating weight A 641/A 641M Speciﬁcation for Zinc-Coated (Galvanized) for each wire size.) Carbon Steel Wire2 4.4.2 For Coating Type Z, see Table 2. A 700 Practices for Packaging, Marking, and Loading 4.4.3 For Coating Type AZ, see Table 3. Methods for Steel Products for Domestic Shipment3 4.5 Grades: A 809 Speciﬁcation for Aluminum-Coated (Aluminized) 4.5.1 Standard Grade—Barbs spaced on 4 or 5-in. (102 or Carbon Steel Wire2 127-mm) centers as indicated in Table 1. A 856/A 856M Speciﬁcation for Zinc-5 % Aluminum- 4.5.2 High-Security Grade—Barbs spaced on 3-in. (76-mm) Mischmetal Alloy-Coated Carbon Steel Wire2 centers (for Coating Type A only). A 902 Terminology Relating to Metallic Coated Steel Prod- NOTE 1—The design numbers are related to the characteristics of the ucts2 construction of the barbed wire, with the number groups related, in order, 2.2 Federal Standard: to the steel wire gage of the strand wires, number of barb points, spacing Fed. Std. No. 123 Marking for Shipments (Civil Agencies)4 of barbs, steel wire gage of the barbs, and a letter indicating the shape of the barbs. 2.3 Military Standards: 5. Ordering Information 1 This speciﬁcation is under the jurisdiction of ASTM Committee A-5 on 5.1 Orders for material under this speciﬁcation shall includeMetallic-Coated Iron and Steel Products and is the direct responsibility ofSubcommittee A05.12 on Wire Speciﬁcations. the following information, as necessary to describe the desired Current edition approved April 10, 1999. Published July 1999. Originally product.published as A121 – 28T. Last previous edition A121 – 92a. 2 5.1.1 Name of material (steel barbed wire), Annual Book of ASTM Standards, Vol 01.06. 3 5.1.2 Quantity (number of spools and length of barbed wire Annual Book of ASTM Standards, Vol 01.05. 4 Available from Standardization Documents Order Desk, Bldg. 4 Section D, 700 on each, or total length) (see 7.5 for standard size of spools),Robbins Ave., Philadelphia, PA 19111-5094, Attn: NPODS. 5.1.3 Metallic coating type (see 4.3), 1
A 121 TABLE 1 Standard Sizes and Constructions for Barbed Wire Nominal Diameter of Coated Number of Barb Spacing of Barbs, Diameter of Barbs, Steel Design Number Size, Steel Wire Gage Shape of Barbs Wire, in. (mm) Points in. (mm) Wire GageA Metallic Coating Type A 12-4-3-14RB 121⁄2 0.099 (2.51) 4 3 (76) 14 Round 12-4-5-14R 121⁄2 0.099 (2.51) 4 5 (127) 14 Round Metallic Coating Type Z and Type ZA 12-2-4-12F 121⁄2 0.099 (2.51) 2 4 (102) 121⁄2C Flat 12-2-4-13F 121⁄2 0.099 (2.51) 2 4 (102) 13C Flat 12-2-4-14R 121⁄2 0.099 (2.51) 2 4 (102) 14 Round 12-2-5-12F 121⁄2 0.099 (2.51) 2 5 (127) 121⁄2C Flat 12-2-5-14R 121⁄2 0.099 (2.51) 2 5 (127) 14 Round 12-4-5-14H 121⁄2 0.099 (2.51) 4 5 (127) 14C Half-round 12-4-5-14R 121⁄2 0.099 (2.51) 4 5 (127) 14 Round 13-2-4-14R 131⁄2 0.086 (2.18) 2 4 (102) 14 Round 13-4-5-14R 131⁄2 0.086 (2.18) 4 5 (127) 14 Round 15-2-5-13F 151⁄2 0.067 (1.70) 2 5 (127) 133⁄4C Flat 15-2-5-14R 151⁄2 0.067 (1.70) 2 5 (127) 14 Round 15-4-5-16R 151⁄2 0.067 (1.70) 4 5 (127) 161⁄2 Round A The nominal diameter of the wire used in making the barbs shall be as follows: 121⁄2 gage 0.099 in. (2.51 mm) 13 gage 0.092 in. (2.32 mm) 133⁄4 gage 0.083 in. (2.11 mm) 14 gage 0.080 in. (2.03 mm) 161⁄2 gage 0.058 in. (1.47 mm) B Design Number 12–4–3–12R, Metallic Coated Type A, is High-Security Grade. All other design numbers are for standard grade. C The gage of the half-round and ﬂat barbs is designated by the gage of the round wire from which the barbs are rolled. TABLE 2 Minimum Weight of Coating on Type Z Barbed Wire wire, 20 spools of 80 rods each, Coating Type Z, Coating Class 3, Design Minimum Weight of Number 12-2-4-14R, to ASTM Speciﬁcation A 121-99, with certiﬁcation. Nominal Diameter ofSize, Steel Coating of Uncoated Wire Type Z Surface, oz/ft2(g/m2) 5.2 All spools of barbed wire accepted by the purchaserWire Gage shall be billed on the basis of the original length of the spools in. (mm) Class 1 Class 3 before sampling, unless changed by contractual agreement. 12 ⁄ 12 0.099 (2.51) 0.28 (85) 0.80 (245) 13 0.092 (2.32) 0.28 (85) 0.75 (230) 131⁄2 0.086 (2.18) 0.25 (75) 0.70 (215) 6. Material A 133⁄4 0.083 (2.11) 0.70 (215) 14 0.080 (2.03) 0.25 (75) 0.70 (215) 6.1 Base Metal—The base metal of the steel strand wires 151⁄2 0.067 (1.70) A 0.65 (200) and steel barbs shall be of good commercial quality carbon A 161⁄2 0.058 (1.47) 0.60 (200) steel, capable of meeting the breaking strength requirement in A These sizes only furnished with Class 3 Coating (Section 8). 7.7. The base metal for aluminum barbs (permitted with metallic Coating Type A) shall be aluminum alloy wire TABLE 3 Minimum Weight of Coating on Type ZA Barbed Wire conforming to Alloy 5000-H38, Alloy 6061-T94, or equal. Nominal Diameter Minimum Weight of Coating of Uncoated 6.1.1 For Coating Type A barbed wire, the choice of whetherSize Wire of Type ZA Wire Wire Surface, oz/ft2(g/m2) ClassA aluminum-coated steel wire or aluminum alloy wire for the Gage in. (mm) 20 40 60 80 100 120 barbs shall be that of the manufacturer, unless otherwise 121⁄2 0.099 (2.51) XB X X X X X speciﬁed by the purchaser. If aluminum alloy wire is used, the 13 0.092 (2.32) X X X X X X particular alloy shall be agreed upon between the manufacturer 131⁄2 0.086 (2.18) X X X X X X 133⁄4 0.083 (2.11) X X X X X X and the purchaser at the time the order is placed. 14 0.080 (2.03) X X X X X X 6.2 Coating Materials—The coating on the wire shall con- 151⁄2 0.067 (1.70) X X X X X X form with the requirements of the following speciﬁcations: 161⁄2 0.058 (1.47 X X X X X X 6.2.1 Coating Type A—Aluminum-coated wire in accor- A Coating Class 20 40 60 80 100 120 dance with Speciﬁcation A 809. Coating Weight oz/ft2 0.20 0.40 0.60 0.80 1.00 1.20 6.2.2 Coating Type Z—Zinc-coated wire in accordance with (g/m)2 61 122 183 244 305 366 Speciﬁcation A 641/A 641M. B X denotes availability. 6.2.3 Coating Type ZA—Zinc-5 % aluminum-mischmetal alloy (Zn-5Al-MM) coated wire in accordance with Speciﬁca- 5.1.4 Metallic coating class (for Types Z and ZA) (see Table tion A 856/A 856M.2 or Table 3), 6.3 Coated Wire—The steel wire shall be coated before 5.1.5 Design Number (see Table 1), fabrication. 5.1.6 For Coating Type A barbed wire, whether aluminum 6.3.1 Weight of Coating Requirements for Strand Wires—alloy barbs are required or prohibited (see 6.2.1). If not stated, The strand wires for Types Z and ZA barbed wire, asthe choice shall be at the manufacturer’s option, represented by the test specimens, shall conform to the 5.1.7 ASTM designation and year of issue, and requirements of Tables 2 and 3 respectively for the minimum 5.1.8 Certiﬁcation or test report, or both, if required. coating weight for the type and class ordered. The strand wires NOTE 2—A typical ordering description is as follows: Steel barbed for Type A barbed wire, as represented by the test specimens, 2
A 121shall have a minimum coating weight of 0.30 oz/ft2(90 g/m2) 8.2.2 A sample length of 25 ft (7.6 m) of barbed wireon the 121⁄2–gage wire. contains: 6.3.2 Weight of Coating Requirements for Barbs—The wire 18.104.22.168 A minimum of 86 barbs for 3-in. (76-mm) spacing,for barbs for Types Z and ZA barbed wire, as represented by 22.214.171.124 A minimum of 69 barbs for 4-in. (102-mm) spacing,the test specimens, shall conform to the same coating class orrequirements as the strand wire. The steel wire for barbs for 126.96.36.199 A minimum of 55 barbs for 5-in. (127-mm) spacing.Type A barbed wire, as represented by the test specimens, shallhave a minimum coating weight of 0.25 oz/ft2(75 g/m2) on the 9. Sampling and Testing14–gage wire. 9.1 Sampling—For the purpose of tests, select one spool at random from every 50 spools or fraction thereof in a lot, or a7. General Requirements total of seven samples, whichever is less. A lot shall consist of 7.1 The sizes and constructions for barbed wire furnished all spools of a single construction (Design Number) of barbedunder this speciﬁcation shall be in accordance with the wire offered for delivery at the same time.requirements of Table 1 for the Design Number speciﬁed in the 9.2 Test Specimens for Physical Tests—Cut a 4-ft (1.2-m)order, within the tolerances stated in Section 8. length of barbed wire from the end of each spool for tests 7.2 The barbs shall be sharp, well-formed, and tightly prescribed in Sections 6 and 7. Determine the breaking strengthwrapped. The barb length, measured from the center of the two value by testing the twisted strand as composite. Test eachstrand wires, shall be 3⁄8 in. (9.5 mm) minimum. strand wire individually for weight of coating. 7.3 The strand wires shall be twisted with a uniform length 9.3 Testing for Weight of Coating—Coating weight forof lay. Type Z and Type ZA barbed wire shall have the twisting Types Z and ZA shall be determined in accordance with Testconsistently in one direction (left or right) or alternating Method A 90/A 90M. Coating weight for Type A shall bebetween the left and right directions. Type A barbed wire shall determined in accordance with Test Method A 428/A 428M.have the twisting consistently in either the left or right Perform testing either before or after fabrication for the stranddirection, with alternating of the twisting prohibited. wires and for Type A steel barbs. Perform testing prior to 7.4 Splicing of individual wires by means of a wrap joint or fabrication for Type Z and ZA barbs, and certify the test results.an electric butt weld is permitted. Not more than three splices 9.4 Pretesting of Wire—Instead of testing wire for breakingor joints shall exist in any spool of barbed wire. Such splices or strength and weight of coating from the completed barbed wirejoints shall be made in a workmanlike manner. in accordance with 9.2, the manufacturer, at his election, shall establish compliance with the requirements in Sections 6 and 7 7.5 The barbed wire, for the various types, shall be pack- by tests made on wire prior to fabrication. If the manufactureraged on spools in lengths as follows: makes this election, the purchaser still has the right to test wire 7.5.1 Type A—80 rods (1320 ft) (402 m) or 1000 ft (305 m). from the completed barbed wire for compliance. It is recog- 7.6 Types Z and ZA—80 rods (1320 ft) (402 m) or 80 rods nized that during fabrication the barb is mechanically deformedplus additional increments of 10 rods (165 ft) (50 m). and scraped, and some differences are likely in coating weight 7.7 Breaking Strength—The breaking strength of the results on barbs tested before and after fabrication.stranded barbed wire, for all types, shall be not less than 950 9.5 Inspection for General Workmanship—For the purposelbf (4230 N). This breaking strength reﬂects that of both strand of inspection, a maximum of two spools from the lot, aswires tested together as one unit. described in 9.1, shall be subjected to observations for barb length and spacing, overall length, and workmanship.8. Permissible Variations in Dimensions 9.5.1 Instead of inspecting for length by unrolling full 8.1 Diameter—The permissible variation from the nominal spools, the purchaser and manufacturer have the option ofdiameter of the wire, for both line wires and barbs, for all agreeing on a weight per spool related to wire size ortypes, shall be 60.005 in. (0.13 mm) measuring tools employed during manufacturing. The pur- 8.1.1 Due to the mechanics of manufacture when forming chaser still reserves the right to conﬁrm the length by actualthe barbs, a certain amount of out-of-roundness is expected. measurement.The size and condition precludes barbs from being subjected to 9.5.2 Inspection for barb spacing is normally performed ondiameter checks. the outer 25-ft (7.6-m) length of a spool, which permits 8.2 Barb Spacing—The nominal spacing of the barbs shall repacking of the spool. Any other selection shall be as agreedbe as noted in Table 1. The individual barb spacing shall be upon between the manufacturer and the purchaser.measured from the edge of one barb at the strand to thecorresponding edge of the adjacent barb. Cumulative spacing is 10. Retestsestablished by counting the total number of barbs in a 25-ft 10.1 Lot Size for Retests—If one or more of the individual(7.6-m) length of barbed wire. Barbs are subject to relocation wire specimens fail the coating weight, or if a strand specimenduring fabrication and handling, potentially leading to rejec- fails the breaking strength test, the lot shall be subject to retest.tions with rigid interpretation of the spacing requirement. For retest purposes, four additional spools of barbed wire forTherefore, barb spacing shall be considered acceptable under each 50 spools offered shall be sampled. The lot size thenthe following conditions: becomes 50 spools, except variation in lot size is permitted to 8.2.1 The sample has 93.5 % of the individual barb spacings accommodate pallet count when the barbed wire is palletized.conforming to the speciﬁed spacing 63⁄4 in. (19 mm), and 10.2 Retesting for Coating Weight—If more than two of the 3
A 121individual strand wires of the retest specimens fail to meet the of dissatisfaction with the results of the test, the manufacturerrequirements of 6.3, or if any of the retest specimens has less or supplier shall make claim for a rehearing.than 75 % of the speciﬁed coating weight, the entire lot 12.2 Instead of rejecting the entire lot as provided in Sectionrepresented by the retest shall be rejected. 10, the manufacturer has the option of testing specimens from 10.3 Retesting for Breaking Strength—If any of the retest every spool and rejecting only those spools failing the weightspecimens fail to meet the minimum breaking strength value in of coating or breaking strength requirements.7.7, the entire lot represented by the specimens shall be 13. Certiﬁcationrejected. 10.4 Reinspection for Barb Spacing, Barb Length, and 13.1 When speciﬁed in the purchase order or contract, aOverall Length—If either of the sample spools fails to meet the manufacturer’s or supplier’s certiﬁcation stating that the ma-requirements for these dimensions, within the tolerances in terial was manufactured, sampled, tested, and inspected inSection 8, two additional spools shall be selected for inspec- accordance with this speciﬁcation and has been found to meettion. If either of these spools fails to meet the requirements, the the requirements shall be furnished to the purchaser. Whenlot shall be rejected. speciﬁed in the purchase order or contract, a report of the test results shall be furnished.11. Inspection 14. Packing and Package Marking 11.1 Unless otherwise speciﬁed in the purchase order or 14.1 Unless otherwise speciﬁed, packaging, marking, andcontract, the manufacturer is responsible for the performance loading for shipment shall be in accordance with Practicesof all inspection and test requirements speciﬁed in this speci- A 700.ﬁcation. Except as otherwise speciﬁed in the purchase order or 14.2 When speciﬁed in the contract or order, and for directcontract, the contractor shall use his own or any other suitable shipment to the U.S. Government, when Level A is speciﬁed,facilities for the performance of the inspection and test preservation, packaging, and packing shall be in accordancerequirements unless disapproved by the purchaser at the time with Level A requirement of MIL-STD-163.the order is placed. The purchaser shall have the right to 14.3 When speciﬁed in the contract or order, and for theperform any of the inspections and tests set forth in this direct procurement by or direct shipment to the U.S. Govern-speciﬁcation when such inspections and tests are deemed ment, marking for shipment, in addition to the requirementsnecessary to ensure that the material conforms to the prescribed speciﬁed in the contract or order, shall be in accordance withrequirements. MIL-STD-129 for U.S. military agencies and in accordance12. Rejection and Rehearing with Fed. Std. No. 123 for U.S. Government civil agencies. 12.1 Material that fails to conform to the requirements of 15. Keywordsthis speciﬁcation shall be rejected. Rejection shall be reported 15.1 barbed wire; carbon steel wire; metallic coated steelto the manufacturer or supplier promptly and in writing. In case wire; steel barbed wire; wire The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, 100 Barr Harbor Drive, West Conshohocken, PA 19428. 4